and long luminescence lifetimes. However, lanthanide emissions are difficult to sensitize directly because they must undergo LaPorte forbidden f-f transitions. Indirect sensitization of lanthanide emission can be accomplished by employing the "antenna effect", where the organic linkers act as antennae and absorb the excitation energy, transfer the energy to the excited state of the lanthanide, and yield lanthanide luminescence upon relaxation. A prime example of the antenna effect is demonstrated by MOF-76, which combines trivalent lanthanide ions and 1,3,5-benzenetricarboxylate (BTC) linkers to form infinite rod SBUs coordinated into a three dimensional lattice. As demonstrated by multiple research groups, the BTC linker can effectively sensitize the lanthanide emission, resulting in a MOF with variable emission wavelengths depending on the lanthanide identity. Additionally, the Yan group has shown that Eu3+- and Tb3+- MOF-76 can be used for selective detection of acetophenone from other volatile monoaromatic hydrocarbons. Upon acetophenone uptake, the MOF shows a very sharp decrease, or quenching, of the luminescence intensity. For use in biological imaging, however, two main obstacles must be overcome: MOFs must be synthesized on the nanoscale so as not to affect the target's normal interactions or behavior The absorbance and emission wavelengths must occur in regions with minimal overlap from sample autofluorescence, other absorbing species, and maximum tissue penetration. Regarding the first point, nanoscale MOF (NMOF) synthesis has been mentioned in an earlier section. The latter obstacle addresses the limitation of the antenna effect. Smaller linkers tend to improve MOF stability, but have higher energy absorptions, predominantly in the ultraviolet (UV) and high-energy visible regions. A design strategy for MOFs with redshifted absorption properties has been accomplished by using large, chromophoric linkers. These linkers are often composed of polyaromatic species, leading to large pore sizes and thus decreased stability. To circumvent the use of large linkers, other methods are required to redshift the absorbance of the MOF so lower energy excitation sources can be used. Post-synthetic modification (PSM) is one promising strategy. Luo et al. introduced a new family of lanthanide MOFs with functionalized organic linkers. The MOFs, deemed MOF-1114, MOF-1115, MOF-1130, and MOF-1131, are composed of octahedral SBUs bridged by amino functionalized dicarboxylate linkers. The amino groups on the linkers served as sites for covalent PSM reactions with either salicylaldehyde or 3-hydroxynaphthalene-2-carboxyaldehyde. Both of these reactions extend the π-conjugation of the linker, causing a redshift in the absorbance wavelength from 450 nm to 650 nm. The